The term machinability
refers to the ease with which a metal can be machined
to an acceptable surface finish. Materials with good machinability require little power to cut, can be cut quickly, easily obtain a good finish, and do not wear the tooling much; such materials are said to be free machining. The factors that typically improve a material's performance often degrade its machinability. Therefore, to manufacture components economically, engineers are challenged to find ways to improve machinability without harming performance.
Machinability can be difficult to predict because machining has so many variables. In most cases, the strength and toughness of a material are the primary factors. Strong, tough materials are usually more difficult to machine simply because greater force is required to cut them. Other important factors include the chemical composition, thermal conductivity and microstructure of the material, the cutting tool geometry, and the machining process parameters. Sometimes, especially for non-metals, the ancillary factors are most important. For example, soft materials like plastics can be difficult to machine because of their poor thermal conductivity.
There are many factors affecting machinability, but no widely accepted way to quantify it. Instead, machinability is often assessed on a case-by-case basis, and tests are tailored to the needs of a specific manufacturing process. Common metrics for comparison include tool life, surface finish, cutting temperature, and tool forces and power consumption.
Tool life method
Machinability can be based off of the measure of how long a tool lasts. This can be useful when comparing materials that have similar properties and power consumptions, but one is more abrasive and thus decreases the tool life. The major downfall with this approach is that tool life is dependent on more than just the material is it machining; other factors include cutting tool material, cutting tool geometry, machine condition, cutting tool clamping, cutting speed, feed, and depth of cut. Also, the machinability for one tool type cannot be compared to another tool type (i.e. HSS
tool to a carbide tool).
Tool forces and power consumption method
The forces required for a tool to cut through a material is directly related to the power consumed. Therefore, tool forces are often given in units of specific energy. This leads to a rating method where higher specific energies equal lower machinability. The advantage of this method is that outside factors have little effect on the rating.
Surface finish method
The surface finish is sometimes used to measure the machinability of a material. Soft, ductile materials tend to want to form a built up edge
. Stainless steel and other materials with a high strain hardening
ability also want to form a built up edge. Aluminium alloys, cold worked steels, and free machining steels, as well as materials with a high shear zone don't tend to form built up edges, so these materials would rank as more machinable.
The advantage of this method is that it is easily measured with the appropriate equipment. The disadvantage of this criterion is that it is often irrelevant. For instance when making a rough cut, the surface finish is of no importance. Also, finish cuts often require a certain accuracy that naturally achieves a good surface finish. This rating method also doesn't always agree with other methods. For instance titanium alloys would rate well by the surface finish method, low by the tool life method, and intermediate by the power consumption method.
The machinability rating of a material attempts to quantify the machinability of various materials. It is expressed as a percentage or a normalized value
. The American Iron and Steel Institute
(AISI) determined machinability ratings for a wide variety of materials by running turning tests at 180 surface feet per minute
(sfpm). It then arbitrarily assigned 160 Brinell B1112 steel a machinability rating of 100%. The machinability rating is determined by measuring the weighed averages of the normal cutting speed, surface finish, and tool life for each material. Note that a material with a machinability rating less than 100% would be more difficult to machine than B1112 and material with a value more than 100% easier.
Machinability ratings can be used in conjunction with the Taylor tool life equation, , in order to determine cutting speeds or tool life. It is known that B1112 has a tool life of 60 minutes at a cutting speed of 1000 sfpm. If a material has a machinability rating of 70%, it can be determined, with the above knowns, that in order to maintain the same tool life (60 minutes) the cutting speed must be 70 sfpm (assuming the same tooling is used).
The carbon content of steel greatly affects its machinability. High-carbon steels are difficult to machine because they are tough and because they may contain carbides that abrade the cutting tool. On the other end of the spectrum, low-carbon steels are troublesome because they are too soft. Low-carbon steels are "gummy" and stick to the cutting tool, resulting in a built up edge
that shortens tool life. Therefore, steel has the best machinability with medium amounts of carbon, about 0.20%.
Chromium, molybdenum and other alloying metals are often added to steel to improve its strength. However, most of these metals also decrease machinability.
Inclusions in steel, especially oxides, may abrade the cutting tool. Machinable steel should be free of these oxides.
There are a variety of chemicals, both metal and non-metal, that can be added to steel to make it easier to cut. These additives may work by lubricating the tool-chip interface, decreasing the shear strength of the material, or increasing the brittleness of the chip. Historically, sulphur and lead have been the most common additives, but bismuth and tin are increasingly popular for environmental reasons.
Lead can improve the machinability of steel because it acts as an internal lubricant in the cutting zone. Since lead has poor shear strength, it allows the chip to slide more freely past the cutting edge. When it is added in small quanities to steel, it can greatly improve its machinability while not significantly affecting the steel's strength.
Sulphur improves the machinability of steel by forming low shear strength inclusions in the cutting zone. These inclusions are stress risers that weaken the steel, allowing it to deform more easily.
Stainless steels have poor machinability compared to regular carbon steel because they are tougher, gummier and tend to work harden very rapidly. Slightly hardening the steel may decrease its gumminess and make it easier to cut. AISI grades 303 and 416 are easier to machine because of the addition of sulphur and phosphorus.
Aluminum is much softer than steel, and techniques to improve its machinability usually rely on making it more brittle. Alloys 2007, 2011 and 6020 have especially good machinability.
are difficult to machine because they have poor thermal conductivity. This creates heat that builds up in the cutting zone, which degrades the tool life and locally melts the plastic. Once the plastic melts, it just flows around the cutting edge instead of being removed by it. Machinability can be improved by using high lubricity coolant and keeping the cutting area free of chip build up.
often have the worst machinability because they combine the poor thermal conductivity of a plastic resin with a tough or abrasive ceramic matrix.
The machinability of rubber
and other soft materials improves by using a very low temperature coolant, such as liquid carbon dioxide. The low temperatures chill the material prior to cutting so that it is more brittle and requires less energy to machine.